Structural diversities in Cu(i) and Ag(i) sulfonate coordination polymers and their anion exchange properties
Singh, Suryabhan; Karthik, Rajendran; CrystEngComm 17 (2015) 7363–; doi:10.1039/C5CE01452B

data_7221789
_publ_section_title
;
 Structural diversities in Cu(i) and Ag(i) sulfonate coordination polymers
 and their anion exchange properties
;
_journal_issue                   38
_journal_name_full               CrystEngComm
_journal_page_first              7363
_journal_paper_doi               10.1039/C5CE01452B
_journal_volume                  17
_journal_year                    2015
_chemical_formula_sum            'C15 H12 Ag N2 O5 S'
_chemical_formula_weight         440.20
_space_group_crystal_system      monoclinic
_space_group_IT_number           11
_space_group_name_Hall           '-P 2yb'
_space_group_name_H-M_alt        'P 1 21/m 1'
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014
_audit_update_record
;
2015-05-18 deposited with the CCDC.
2015-08-13 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 98.79(2)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.399(3)
_cell_length_b                   18.503(6)
_cell_length_c                   12.632(5)
_cell_measurement_temperature    293(2)
_cell_volume                     1709.1(11)
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.994
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1722
_diffrn_reflns_av_unetI/netI     0.2557
_diffrn_reflns_laue_measured_fraction_full 0.997
_diffrn_reflns_laue_measured_fraction_max 0.994
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       23
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            13793
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.994
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.551
_diffrn_reflns_theta_min         1.631
_exptl_absorpt_coefficient_mu    1.328
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            'Light yellow'
_exptl_crystal_density_diffrn    1.711
_exptl_crystal_description       Rectangular
_exptl_crystal_F_000             876
_exptl_crystal_recrystallization_method 'Water and methanol'
_exptl_crystal_size_max          0.34
_exptl_crystal_size_mid          0.32
_exptl_crystal_size_min          0.30
_refine_diff_density_max         1.237
_refine_diff_density_min         -0.937
_refine_diff_density_rms         0.155
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.918
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     244
_refine_ls_number_reflns         4047
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.918
_refine_ls_R_factor_all          0.2800
_refine_ls_R_factor_gt           0.0931
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1248P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2080
_refine_ls_wR_factor_ref         0.2860
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1298
_reflns_number_total             4047
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c5ce01452b2.cif
_cod_data_source_block           shelx
_cod_depositor_comments
'Adding full bibliography for 7221785--7221790.cif.'
_cod_database_code               7221789
_shelxl_version_number           2014-3
_shelx_res_checksum              79374